The fluoride ion has a well-established beneficial role in dentistry in protecting the teeth from assault by caries. It is known to contribute to the dynamic mineralisation process of the natural tooth mineral, and also to become incorporated with the mineral phase, forming a thin layer of fluorapatite. This is more resistant to acid attack than the native hydroxyapatite, hence protects the tooth against further decay. Other recently discovered aspects of the role and uptake of fluoride will also be discussed.
One of the widely used dental restoratives, the glass-ionomer dental cement, is able to release fluoride in a sustained manner that may continue for many years, and this is seen as clinically beneficial. The closely related resin-modified glass-ionomer cement, and also the polyacid-modified composite resin (“compomer”) are able to do the same. There are also fluoride-containing conventional composite resins able to release fluoride.
These various materials are reviewed and the way in which they release fluoride are described, as well as the effectiveness of the release at the levels involved. Studies of effectiveness of fluoride release from these various classes of material are reviewed, and shown to suggest that release from conventional and resin-modified glass-ionomers is more beneficial than from composite resins. This is attributed to 2 causes: firstly, that it is not possible to replace the lost fluoride in composites, unlike glass-ionomers, and secondly because the other ions released from glass-ionomers (calcium, phosphate) are able to contribute to local remineralisation of the tooth. The absence of these other ions in fluoridated composites means that remineralisation is able to occur to a lesser extent, if at all.
*Presented at the 19th Congress of the BaSS, Belgrade, 2014
6. ten Cate JM. Contemporary perspective on the use of fluoride products in caries prevention. Br Dent J, 2013; 214:161-167.
7. ten Cate JM, Featherstone JD. Mechanistic aspects of the interactions between fluoride and dental enamel. Crit Rev Oral Biol Med, 1991; 2:283-296.
8. ten Cate JM, Buijs MJ, Miller CC, Exterkate RA. Elevated fluoride products enhance mineralisation of advanced enamel lesions. J Dent Res, 2008; 87:943-947.
9. Fejerskow O, Kidd EAM (eds). Dental caries: The disease and its clinical management, Oxford: Blackwell and Munsgaard, 2008.
10. Hojo S, Takahashi N, Yamada T. Acid profile in carious dentin. J Dent Res, 1991; 70:182-186.
11. Larsen MJ, Fejerskov O. Chemical and structural challenges in remineralization of dental enamel lesions. Scand J Dent Res, 1989; 97:285-296.
12. Cury JA, Tenuta LMA. Enamel remineralization: controlling the caries disease or treating early caries lesions? Braz J Oral Res, 2009; 23(special issue 1):23-30.
13. Robinson CA, Shore RC, Brookes SJ, Stafford S, Wood SR, Kirkham J. The chemistry of enamel caries. Crit Rev Oral Biol Med, 2000; 11:481-495.
14. de Leeuw NH. Resisting the onset of hydroxyapatite dissolution through the incorporation of fluoride. J Phys Chem B, 2004; 108:1809-1811.
15. Edgar WM, Higham SM. Role of saliva in caries models. Adv Dent Res, 1995; 9:235-238.
16. Yehia A, Ezzat K. Fluoride uptake by synthetic apatites. Adsorption Sci & Technol, 2009; 27:337-347.
17. Tenuta LMA, Cury JA. Fluoride: Its role in dentistry. Braz J Oral Res, 2010; 24(special issue 1):9-17.
18. Fan X, Parker DJ, Smith MD. Adsorption kinetics of fluoride on low cost materials. Water Res, 2008; 37:4929-4937.
19. Gomwe T, Booth SE, Nicholson JW. The kinetics of fluoride uptake by synthetic hydroxyapatite. Ceramics-Silikaty, 2012; 56:85-88.
20. Patniak P. Handbook of Inorganic Chemistry. New York: McGraw-Hill, 2002.
21. Mclean JW, Nicholson JW, Wilson AD. Proposed nomenclature for glass-ionomer dental cements and related materials. Quintessence Int, 1994; 25:587-589.
22. Mount GJ, Tyas MJ, Ferracane J, Nicholson JW, Berg JH, Simonsen RJ, Ngo HC. A revised classification for direct tooth-colored restorative materials. Quintessence Int, 2009; 40:691-697.
23. Breshi I, Mazzoni A, Ruggeri A, Cadenaro M, Lenarda R, De Stafano Dorigo E. Dental adhesion review: aging and stability of bonded surfaces. Dent Mater, 2008; 24:90-101.
24. Furtos G, Cosma V, Prejmerean C, Moldovan M, Brie M, Colceriu M, Vezsenyi L, Silaghi-Dumitrescu L, Sirbu C. Fluoride release from dental resin composites. Mater Sci & Eng C, 2005; 25:231-236.
25. Nicholson JW. Polyacid-modified composite resins (“compomers”) and their use in clinical dentistry. Dent Mater, 2007; 23:615-622.
26. Nicholson JW, Alsarheed M. Changes on storage of polyacid-modified composite resins. J Oral Rehabil, 1998; 25:616-620.
27. Czarnecka B, Limanowska-Shaw H, Nicholson JW. Buffering and ion release by a glass-ionomer cement under near-neutral and acidic conditions. Biomaterials, 2002; 23:2783-2788.
28. Ngo H, Mount GJ, Peters MCRB. A study of glass-ionomer cement and its interface with enamel using a low-temperature, high-resolution scanning electron microscopic technique. Quintessence Int, 1997; 28:63-69.
29. Ngo H, Mount GJ, McIntyre J, Tuisuva J, von Doussa RJ. Chemical exchange between glass ionomer restorations and residual carious dentine in permanent molars: An in vivo study. J Dent, 2006; 4:608-613.
30. Frencken JE. The ART approach using glass-ionomers in relation to global oral health care. Dent Mater, 2010; 26:1-6.
31. Weigand A, Buchalla W, Attin T. Review on fluoride-releasing restorative materials - Fluoride release and uptake characteristics, antibacterial activity and influence on caries formation. Dent Mater, 2007; 23:343-362.
32. Croll TP, Nicholson JW. Glass ionomer cements in pediatric dentistry: review of the literature. Pediatr Dent, 2002; 24:423-429.
33. Mitra SB. Adhesion to dentin and physical properties of a light-cured glass-ionomer liner/base. J Dent Res, 1991; 70:72-74.
34. Mitra SB. In vitro fluoride release from a light-cured glass-ionomer liner/base. J Dent Res, 1991; 70:75-78.
35. Wilson AD. Resin-modified glass-ionomer cements. Int J Prosthodont, 1990; 3:425-429.
36. Nicholson JW, Czarnecka B. The biocompatibility of resin-modified glass-ionomers for dentistry. Dent Mater, 2008; 24:1702-1708.
37. Palmer G, Anstice HM, Pearson GJ. The effect of curing regime on the release of hydroxyethyl methacrylate (HEMA) from resin-modified glass ionomer cements. J Dent, 1999; 27:303-311.
38. Hamid A, Hume WR. The effect of dentine thickness on diffusion of resin monomers in vitro. J Oral Rehabil, 1997; 24:20-25.
39. Geukins S, Goossens A. Occupational contact allergy to (meth)acrylates. Contact Dermatol, 2001; 44:153-159.
40. Katsumo K, Manabe A, Itoh K, Nakamura Y, Wakumoto S, Hisamitsu H, Yoshida T. Contact dermatitis caused by 2-HEMA and GM dentine primer solutions applied to guinea pigs and humans. Dent Mater J, 1996; 15:22-30.
41. Arora V, Bogra P. Giomer: A new hybrid aesthetic restorative material. J Conserv Dent, 2002; 5:149-155.
42. Nakamura N, Yamada A, Iwamoto T, Arakai M, Tanaka K, Aizawa S, Nonaka K, Fukumoto S. Two-year clinical evaluation of flowable composite resin containing pre-reacted glass-ionomer. Ped Dent J, 2009; 19:89-97.
43. Saku S, Kotake H, Scongall-Vilchis RJ, Ohashi S, Hotta M, Horuichi S, Hamada K, Asoaka K, Tanaka E, Yamamoto K. Antibacterial activity of composite resins with glass-ionomer filler particles. Dent Mater J, 2010; 29:193-198.
44. Zainuddin N, Karpukhina N, Law RV, Hill RG. Characterisation of a remineralising glass carbomer® ionomer cement by MAS-NMR spectroscopy. Dent Mater, 2012; 28:1051-1058.
45. Cehreli SB, Tirali RE, Yalcinkaya Z, Cehreli ZC. Microleakage of newly developed glass carbomer cement in primary teeth. Eur J Dent, 2013; 7:15-21.
46. Billington RW, Williams JA, Pearson GJ. Ion processes in glass ionomer cements. J Dent, 2006; 34:544-555.
47. Forsten L. Short- and long-term fluoride release from glass ionomers. Scand J Dent Res, 1991; 99:241-245.
48. Xu X, Burgess JO. Compressive strength, fluoride release and recharge of fluoride-releasing materials. Biomaterials, 2003; 24:2451-2461.
49. Tay WM, Braden M. Fluoride ion diffusion from polyalkenoate (glass-ionomer) cements. Biomaterials, 1988; 9:454-459.
50. Shaw AJ, Carrick T, McCabe JF. Fluoride release from glass-ionomer and compomer materials; 6 month data. J Dent, 1998; 26:355-359.
51. Bell A, Creanor SL, Foye RH, Saunders WP. The effect of saliva on fluoride release by a glass-ionomer filling material. J Oral Rehabil, 1999; 26:407-412.
52. Koch G, Hatibovic-Kofman S. Glass ionomer cements as a fluoride release system in vivo. Swed Dent J, 1990; 14:267-273.
53. Creanor SL, Carruthers LM, Saunders WP, Strang R, Foye RH. Fluoride uptake and release characteristics of glass ionomer cements. Caries Res, 1994; 28:322-328.
54. Perrin C, Persin M, Sarazin J. A comparison of fluoride release from four glass-ionomer cements. Quintessence Int, 1994; 25:603-608.
55. Hörsted-Bindsler P, Larsen MJ. Release of fluoride from conventional and metal-reinforced glass ionomer cements. Scand J Dent Res, 1990; 98:451-455.
56. Ananjo FB, Garcia-Godoy F, Cury JA, Conceicao EN. Fluoride release from fluoride-containing materials. Oper Dent, 1996; 21:185-190.
57. Yap AU, Tham SY, Zhu LY, Lee HK. Short-term fluoride release from various aesthetic restorative materials. Oper Dent, 2002; 27:259-265.
58. Hatibovic-Kofman S, Koch G. Fluoride release from glass ionomer cement in vivo and in vitro. Swed Dent J, 1991; 15:253-258.
59. Walls AWG. Glass polyalkenoate (glass-ionomer) cements: a review. J Dent, 1986; 14:231-236.
60. Preston AJ, Agalmanyi EA, Higham SM, Mair LH. The recharge of esthetic dental restorative materials with fluoride in vitro - two years’ results. Dent Mater, 2003; 19:32-37.
61. Gao W, Smales RJ, Gale MS. Fluoride release/uptake from new glass ionomer cements used with the ART approach. Am J Dent, 2000; 13:201-204.
62. Preston AJ, Higham SM, Agalmanyi EA, Mair LH. Fluoride recharge of aesthetic dental materials. J Oral Rehabil, 1999; 26:936-940.
63. Strother JM, Kohn DH, Dennison JB, Clarkson BH. Fluoride release and re-uptake in direct tooth-coloured restorative materials. Dent Mater, 1998; 14:129-136.
64. De Witte AM, De Maeyer EA, Verbeeck RMH, Martens LC. Fluoride release profiles of mature restorative glass ionomer cements after fluoride application. Biomaterials, 2000; 21:475-482.
65. Hatibovic-Kofman S, Koch G, Eckstrand J. Glass ionomer material as a rechargeable fluoride release system. Int J Paediatr Dent, 1997; 7:67-73.
66. Diaz-Arnold AM, Holmes DC, Wistrom DW, Swift EJ Jr. Short-term fluoride release/uptake of glass ionomer restoratives. Dent Mater, 1995; 11:96-101.
67. Rothwell M, Anstice HM, Pearson GJ. The uptake and release of fluoride by ion-leaching cements after exposure to toothpaste. J Dent, 1998; 26:591-597.
68. Creanor SL, Saunders WP, Carruthers LM, Strang R, Foye RH. Effects of intrinsic fluoride concentration on the uptake and release of fluoride from two glass ionomer cements. Caries Res, 1995; 29:424-426.
69. Pawluk K, Booth SE, Coleman NJ, Nicholson JW. The kinetics of fluoride uptake from aqueous solutions of immature glass-ionomer dental cements. Dental Forum, 2008; 36:11-14.
70. Nicholson JW, Czarnecka B. Maturation affects fluoride uptake by glass-ionomer dental cements. Dent Mater, 2012; 28:e1-e5.
71. Kantovotz KR, Pascon FM, Correr GM, Alonso RCB, Rodrigues LKA, Alves MC, Puppin-Pontani RM. Influence of environmental conditions on properties of ionomeric and resin sealant materials. J Appl Oral Sci, 2009; 17:294-300.
72. Forss H. Release of fluoride and other elements from light-cured glass ionomers in neutral and acidic conditions. J Dent Res, 1993; 72:1257-1262.
73. Czarnecka B, Nicholson JW. Ion release by resin-modified glass-ionomer cements into water and lactic acid solutions. J Dent, 2006; 34:539-543.
74. Hojo S, Komatsu M, Okuda R, Takahashi N, Yamada T. Acid profiles and pH of carious dentin in active and arrested lesion. J Dent Res, 1994; 73:1853-1857.
75. Corbillon MS, Olazabal MA, Madraiago JM. Potentiometric study of aluminium-fluoride complexation equilibria and definition of the thermodynamic model. J Solution Chem, 2008; 37:567-579.
76. Jackson GE. The existence of AlF4− in aqueous solution and its relevance to phosphorylase reactions. Inorg Chim Acta, 1988; 151:273-276.
77. Lewis SM, Coleman NJ, Booth SE, Nicholson JW. Interaction of fluoride complexes derived from glass-ionomer cements with hydroxyapatite. Ceramics-Silikaty, 2013; 57:196-200.
78. Braden M, Causton BE, Clarke RL. Diffusion of water in composite resins. J Dent Res, 1976; 55:730-732.
79. Adusei GO, Deb S, Nicholson JW. The role of the ionomer glass component in polyacid-modified composite resin dental restorative materials. J Mater Sci Mater Med, 2004; 15:751-754.
80. Karantakis P, Helvatjoglou-Antoniades M, Theodoridou-Pahini S. Fluoride release from three glass ionomers, a compomer and a composite resin in water, artificial saliva and lactic acid. Oper Dent, 2000; 25:20-25.
81. Preston AJ, Mair LH, Agalamanyi EA, Higham, SM. Fluoride release from aesthetic dental materials. J Oral Rehabil, 1999; 26:123-129.
82. Ling L, Xu X, Choi G-Y, Bilodeaux D, Guo G, Diwan RM. Novel F-releasing composite with improved mechanical properties. J Dent Res, 2009; 88:83-88.
83. Cohen BJ, Deutsch AS, Musiant BL. Fluoride release from four reinforced composite resins: a one year study. Oral Health, 1995; 85:7-8.
84. Dijkman GEHM, de Vries J, Loding A, Arends J. Long-term fluoride release of visible light-activated composites in vitro: A correlation with in situ demineralisation data. Caries Res, 1993; 27:117-123.
85. Glasspoole EA, Erickson RL, Davidson CL. A fluoride-releasing composite for dental applications. Dent Mater, 2001; 17:127-133.
86. Yip HK, Smales RJ. Fluoride release from a polyacid-modified resin composite and 3 resin-modified glass-ionomer materials. Quintessence Int, 2000; 31:261-266.
87. Yip HK, Smales RJ. Fluoride release and uptake by aged resin-modified glass ionomers and a polyacid-modified resin composite. Int Dent J, 1999; 49:217-225.
88. Asmussen E, Peutzfeldt A. Long-term fluoride release from a glass ionomer cement, a compomer, and from experimental resin composites. Acta Odontol Scand, 2002; 60:93-97.
89. Itota T, Carrick TE, Yoshiyama M, McCabe JF. Fluoride release and recharge in giomer, compomer and resin composite. Dent Mater, 2004; 20:789-795.
90. Dionysopoulos D, Koliniotou-Koumpia E, Helvatzoglou-Antoniades M, Konstantos N. Fluoride release and recharge abilities of contemporary fluoride-containing restorative materials and dental adhesives. Dent Mater J, 2013; 32:296-300.
91. Van Loveren C, Moore WR, Buijs MJ, van Palenstein Helderman WH. Total and free fluoride in toothpastes from some non-established market economy countries. Caries Res, 2005; 39:224-230.
92. Duckworth RM, Morgan SN. Oral fluoride retention after use of fluoride dentifrices. Caries Res, 1991; 25:123-129.
93. Kumar JV. Is water fluoridation still necessary? Adv Dent Res, 2008; 20:8-12.
94. Duckworth RM, Morgan SN, Murray AM. Fluoride in saliva and plaque following use of fluoride-containing mouthwashes. J Dent Res, 1987; 66:1730-1734.
95. Featherstone JDB, Zero DT. Laboratory and human studies to elucidate the mechanics of action of fluoride-containing dentifrices. In: Embery G, Rølla G (eds). Clinical and biological aspects of dentifrices. Oxford: University Press, 1992; pp 41-50.
96. Benelli EM, Serra MC, Rodrigues Jr AL, Cury JA. In situ anticariogenic potential of glass ionomer cement. Caries Res, 1993; 27:280-284.
97. van Dijken JW, Kalfas S, Litra V, Oliveby A. Fluoride and mutans streptococci levels in plaque on aged restorations of resin-modified glass ionomer cement, compomer andresin composite. Caries Res, 1997; 31:379-383.
98. Seppa L, Salmenkivi S, Forss H. Enamel and plaque fluoride following glass ionomer application in vivo. Caries Res, 1992; 26:340-344.
99. Forss H, Jokinen J, Spets-Happonen S, Seppa L, Luoma H. Fluoride and mutans streptococci in plaque grown on glass ionomer and composite. Caries Res, 1991; 25:454-458.
100. ten Cate JM, Featherstone JDM. Physicochemical aspects of fluoride-enamel interactions. In: O. Fejerskov, J. Ekstrand, BA Burt (eds). Fluoride in dentistry. Copenhagen: Munksgaard, 1996; pp 252-272.
101. Rølla G, Øgaard B, Cruz RA. Topical application of fluorides on teeth. New concepts of mechanisms of interaction. J Clin Periodontol, 1993; 20:105-108.
102. Kawai K, Tantbirojn D, Kamalawat AS, Hasegawa T, Retief DH. In vitro enamel and cementum fluoride uptake from three fluoride-containing composites. Caries Res, 1998; 32:463-469.
103. Eronat N, Kocatas N, Alpoz AR. A comparative study of fluoride uptake from dentin bonding agents and glass-ionomer cements in permanent and primary tooth enamel. Quintessence Int, 1999; 30:496-500.
104. Yamamoto H. Iwami Y, Unezaki T, TomiiY, Tuchitani Y. Fluoride uptake around cavity walls; two-dimensional mapping by electron probe microanalysis. Oper Dent, 2000; 25:104-112.
105. Retief DH, Bradley EL, Denton JC, Switze PR. Enamel and cementum fluoride uptake from a glass ionomer cement. Caries Res, 1984; 18:250-257.
106. Souganidis DJ, Athanassouli TM, Papastathopoulos DS. A study of in vivo fluoride uptake by dental tissues from fluoride-containing silver amalgams. J Dent Res, 1981; 60:105-108.
107. Tarn LE, Chan GP, Yim D. In vitro caries inhibition effects by conventional and resin-modified glass-ionomer restorations. Oper Dent, 1997; 22:4-14.
108. Wesenberg G, Hals E. The structure of experimental in vitro lesions around glass ionomer cement restorations in human teeth. J Oral Rehabil, 1980; 7:175-184.
109. Gjorgievska ES, Nicholson JW, Slipper IJ, Stevanovic MM. Remineralization of demineralized enamel by toothpastes: A scanning electron microscopy, energy dispersive X-ray analysis, and three-dimensional stereo-micrographic study. Microsc Microanal, 2013; 19:587-595.
110. Dijkman GE, Arends J. Secondary caries in situ around fluoride-releasing light-curing composites: a quantitative model investigation on four materials with a fluoride content between 0 and 26 vol%. Caries Res, 1992; 26:351-357